Structural characterization and electrochemical properties of Co3O4 anode materials synthesized by a hydrothermal method
© Shin et al; licensee Springer. 2012
Received: 19 September 2011
Accepted: 9 January 2012
Published: 9 January 2012
Cobalt oxide [Co3O4] anode materials were synthesized by a simple hydrothermal process, and the reaction conditions were optimized to provide good electrochemical properties. The effect of various synthetic reaction and heat treatment conditions on the structure and electrochemical properties of Co3O4 powder was also studied. Physical characterizations of Co3O4 are investigated by X-ray diffraction, scanning electron microscopy, and Brunauer-Emmett-Teller [BET] method. The BET surface area decreased with values at 131.8 m2/g, 76.1 m2/g, and 55.2 m2/g with the increasing calcination temperature at 200°C, 300°C, and 400°C, respectively. The Co3O4 particle calcinated at 200°C for 3 h has a higher surface area and uniform particle size distribution which may result in better sites to accommodate Li+ and electrical contact and to give a good electrochemical property. The cell composed of Super P as a carbon conductor shows better electrochemical properties than that composed of acetylene black. Among the samples prepared under different reaction conditions, Co3O4 prepared at 200°C for 10 h showed a better cycling performance than the other samples. It gave an initial discharge capacity of 1,330 mAh/g, decreased to 779 mAh/g after 10 cycles, and then showed a steady discharge capacity of 606 mAh/g after 60 cycles.
Keywordscobalt oxide hydrothermal method anode material lithium battery
High performance batteries are receiving more attention nowadays, and many battery types are being developed for commercial use. Lithium ion batteries are known to be extremely safe and more reliable than rechargeable batteries with lithium metal because the charge-discharge reaction between a carbon negative electrode and a positive electrode consisting of metal oxide deals only with lithium ion. Research on the anode material for lithium ion battery has been focused on carbonaceous materials and alternative materials like tin oxide, cobalt oxide, etc. . Carbonaceous materials have high stability but low volumetric capacity mainly due to their large initial irreversible capacity. In the last two decades, a number of various insertion compounds have been investigated with respect to their use as possible electrode materials in rechargeable lithium ion batteries.
Transition metal oxides consisting of layered structures or three-dimensional frameworks with tunnel systems accept remarkable amounts of lithium. Nanoscale or micron-sized transition metal oxides are promising alternative anode materials with excellent electrochemical performance for lithium ion batteries. Cobalto-cobaltic oxide belongs to a cubic closely packed structure of oxide ions and has attracted comparatively more attention due to the broad range of applications such as heterogeneous catalysts [2, 3], anode materials in lithium ion rechargeable batteries , solid-state sensors , electrochromic devices , solar energy absorbers [7–9], magnetic materials , and ceramic pigments . Cobalt oxide [Co3O4] is a good candidate as an anode material for lithium secondary batteries because of its good electrochemical capacity and high recharging rate . Various synthetic routes have been developed for the preparation of Co3O4 such as thermal deposition , chemical spray pyrolysis , chemical vapor deposition , pulsed laser deposition , and traditional sol-gel method . These methods need a relatively high temperature, and it is difficult to obtain nanocrystalline Co3O4. However, hydrothermal synthesis has emerged as an attractive and simple route for the preparation of such metal oxide nanoparticles. Jiang et al. reported the hydrothermal synthesis of Co3O4 by a two-step synthetic route using CoSO4·7H2O, ammonia, and H2O2 at 180°C .
In this work, Co3O4 powder was prepared by a hydrothermal process, and the reaction conditions were optimized to provide good electrochemical properties. The effect of various reaction conditions and heat treatment on the structure and electrochemical properties of Co3O4 powder was also studied. Cobalt nitrate hexahydrate (Co(NO3)2·6H2O) as the source of cobalt, hexamethylenetetramine [HMT] (C6H12N4) as a precipitator, and sodium citrate dihydrate (C6H5Na3O7·2H2O) as a template were used for the preparation of Co3O4.
Co3O4 was synthesized by a simple hydrothermal reaction. In a typical procedure, cobalt nitrate hexahydrate, HMT, and sodium citrate dihydrate were added to 100 ml of deionized water with stirring. The mole ratio used for Co(NO3)2:HMT:C6H5Na3O7 was 6:3:2. After stirring for 10 min, the solution was kept in a Teflon-lined stainless steel autoclave and heated to temperatures in the range of 150°C to 250°C for different time durations (6 to 20 h) in a nitrogen atmosphere. The precipitate was collected by centrifugation and washed successively with distilled water and absolute alcohol, and dried at 75°C for 24 h. The precipitate obtained was heated at 200°C to 400°C for 3 h in air.
The characterization of prepared samples was done by X-ray powder diffraction [XRD] (D5005, BRUKER AXS GMBH, Karlsruhe, Germany using an X-ray diffractometer with Cu Kα radiation over the range of 10° to 90° 2θ), and surface morphology was studied using scanning electron microscopy [SEM] (JEOL 5600, JEOL Ltd, Akishima, Tokyo, Japan and TESCAN VEGAIILMU, Czechoslovakia). The specific surface area of the samples was measured using the Brunauer-Emmett-Teller [BET] procedure (ASAP 2010, Micromeritics Instrument Co., Norcross, GA, USA) from the N2 adsorption-desorption isotherms.
The anode was prepared by mixing Co3O4 powder, a carbon conductor (Super P carbon black or acetylene black [AB] (Alfa Aeser, Ward Hill, MA, USA)), and a poly(vinylidene fluoride) (PVdF, Sigma-Aldrich, St. Louis, MO, USA) binder in a 70:20:10 weight ratio. The ingredients were mixed in a high energy mixer mill for 1 h at room temperature using N-methylpyrrolidone as solvent to get a homogenous slurry which was cast on copper foil and dried at 80°C under vacuum for 12 h. The film was cut into circular disks of 1-cm2 area and approximately 1.5-mg mass for use as anode. Electrochemical coin cells were assembled with lithium metal (300 μm in thickness; Cyprus-Foote Mineral Co., Kings Mountain, NC, USA) as cathode, Celgard® 2200 (Celgard LLC, Charlotte, NC, USA) as separator, 1 M LiPF6 in ethylene carbonate/diethyl carbonate (Samsung Cheil Industries, Gyeonggi-do, South Korea; 1:1, v/v) as electrolyte, and Co3O4 as anode. The cell assembly was performed under an argon atmosphere in a glove box (H2O < 10 ppm). The charge-discharge tests were carried out using an automatic galvanostatic charge-discharge unit, WBCS3000 battery cycler, between 0.001 and 2.5 V at a current density of 0.1 C.
Results and discussions
Sodium citrate dihydrate is widely used to make microsphere type particles as a chelate complex and stabilizing agent in nanocolloidal chemistry, which is rendered by three carboxyl anions. These carboxyl anions can adsorb on the surface of metal ions and exert either hydrophobic or coulombic effects on metal ions and thereby act as a template to form and stabilize spherical structures . With the effect of sodium citrate dihydrate, the thickness of layers gradually increases in a concave shape resulting in microsphere formation [19, 20]. The ability of HMT to capture protons might accelerate the formation of crystalline subunits during the gradual hydrolysis of HMT, thereby formation of more amorphous spheres might occur .
The theoretical capacity is 890 mAh/g. The sudden drop in specific capacity of the cell after the first cycle is due to the irreversible reaction of Co3O4. It could be seen that the potential drops rapidly, followed by a plateau at about 1.0 V, and a gradual decrease to the cutoff voltage of 0.001 V for the lithium reaction during the initial discharge process as shown in Figure 4. However, the plateau disappeared during the second cycle. The initial capacities of the cell using AB as the carbon conductor are ordered as follows: the samples prepared at 150°C for 20 h (1,680 mAh/g), 200°C for 10 h (1,420 mAh/g), and 250°C for 8 h (798 mAh/g). All values of the initial capacities of Co3O4 electrodes using Super P and AB carbon conductors were significantly higher than the theoretical capacity. The capacities of the Co3O4 electrode using the Super P carbon conductor decreased rapidly, and the plateau disappeared during the second cycle just like the Co3O4 electrode using AB. In comparison, the cell using AB as conductor delivered a higher initial discharge capacity than the cell using Super P, but the capacity drop is higher in the former.
Figure 6 showed the comparison of cycle performance of the cells based on Co3O4 prepared at 200°C for 10 h and then calcined at different temperatures, 200°C, 300°C, and 400°C, for 3 h. The cells made of Co3O4 calcined at 200°C, 300°C, and 400°C delivered initial discharge capacities of 1,330, 985, and 898 mAh/g which dropped to 677, 279, and 365 mAh/g after 30 cycles, respectively. The sample calcined at 200°C for 3 h showed a better electrochemical property than the other samples which is due to the occurrence of cracks in the samples during high temperature treatment. The sample prepared at 200°C for 3 h has a uniform particle size and high surface area which can provide better sites to accommodate Li+ and electrical contact, and give a good electrochemical property.
Co3O4 particles were synthesized by a simple hydrothermal method at various reaction and heat treatment conditions from cobalt nitrate, hexamethylenetetramine, and sodium citrate dehydrate. Depending on the synthetic conditions, different morphologies were obtained, which noticeably affected the electrochemical properties. The cells with Super P as a carbon conductor showed better electrochemical properties than the cells with AB. The discharge capacity decreased with the increasing cycle number but still remained relatively high. Among the samples prepared under different reaction conditions, Co3O4 prepared at 200°C for 10 h showed a better cycling performance than the other samples.
This research was supported by the World Class University (WCU) program through the National Research Foundation of Korea funded by the Ministry of Education, Science and Technology (grant number: R32-2008-000-20093-0).
- Poizot P, Laruelle S, Grugeon S, Dupont L, Tarascon JM: Searching for new anode materials for the Li-ion technology: time to deviate from the usual path. J Power Sources 2001, 97–98: 235–239.View ArticleGoogle Scholar
- Bailie JF, Rochester CH, Hutching GJ: Effects of thiophene and sulfur dioxide on CO adsorption on cobalt/silica catalysts. J Chem Soc Faraday Trans 1997, 93: 2331–2336. 10.1039/a700803aView ArticleGoogle Scholar
- Schmidtszalowski K, Krawczyk K, Petryk J: The properties of cobalt oxide catalyst for ammonia oxidation. Appl Catal A 1998, 175: 147–157. 10.1016/S0926-860X(98)00206-3View ArticleGoogle Scholar
- Li WY, Xu LN, Chen J: Co3O4Nanomaterials in lithium-ion batteries and gas sensors. Adv Funct Mater 2005, 15: 851–857. 10.1002/adfm.200400429View ArticleGoogle Scholar
- Logothesis EM, Park R, Meitzler AH, Lund KK: Oxygen sensors using CoO ceramics. Appl Phys Lett 1975, 26: 209–212. 10.1063/1.88118View ArticleGoogle Scholar
- Maruyama T, Arai S: Electrochromic properties of cobalt oxide thin films prepared by chemical vapor deposition. J Electrochem Soc 1996, 143: 1383–1386. 10.1149/1.1836646View ArticleGoogle Scholar
- Nozik AJ: Quantum dot solar cells. Physica E 2002, 14: 115–120. 10.1016/S1386-9477(02)00374-0View ArticleGoogle Scholar
- Smith GB, Ignatiev A, Zajac G: Solar selective black cobalt: preparation, structure, and thermal stability. J Appl Phys 1980, 51: 4186–4197. 10.1063/1.328276View ArticleGoogle Scholar
- Chidambaram K, Malhotra KL, Chopra KL: Spray-pyrolysed cobalt black as a high temperature selective absorber. Thin Solid Films 1982, 87: 365–371. 10.1016/0040-6090(82)90289-9View ArticleGoogle Scholar
- Makhlouf SA: Magnetic properties of Co3O4nanoparticles. J Magn Magn Mater 2002, 246: 184–190. 10.1016/S0304-8853(02)00050-1View ArticleGoogle Scholar
- Matijevic E: Preparation and properties of uniform size colloids. Chem Mater 1993, 5: 412–426. 10.1021/cm00028a004View ArticleGoogle Scholar
- Poizot P, Laruelle S, Grugeon S, Dupont L, Tarascon JM: Nano-sized transition-metal oxides as negative-electrode materials for lithium-ion batteries. Nature 2000, 407: 496–499. 10.1038/35035045View ArticleGoogle Scholar
- Trasatti S: Electrodes of Conductive Metallic Oxides Part A. Amsterdam: Elsevier; 1980.Google Scholar
- Singh RN, Koenig JF, Chartier P: Electrochemical studies on protective thin Co3O4and NiCo2O4films prepared on titanium by spray pyrolysis for oxygen evolution. J Electrochem Soc 1990, 137: 1408–1413. 10.1149/1.2086682View ArticleGoogle Scholar
- Fu ZW, Wang Y, Zhang Y, Qin QZ: Electrochemical reaction of nanocrystalline Co3O4thin film with lithium. Solid State Ionics 2004, 170: 105–109. 10.1016/j.ssi.2004.02.020View ArticleGoogle Scholar
- Baydi ME, Poillerat G, Rehspringer JL, Gautier JL, Koenig JF, Chartier P: A sol-gel route for the preparation of Co3O4catalyst for oxygen electrocatalysis in alkaline medium. J Solid State Chem 1994, 109: 281–288. 10.1006/jssc.1994.1105View ArticleGoogle Scholar
- Jiang Y, Wu Y, Xie B, Xie Y, Qian Y: Moderate temperature synthesis of nanocrystalline Co3O4via gel hydrothermal oxidation. Mater Chem Phys 2002, 74: 234–237. 10.1016/S0254-0584(01)00463-1View ArticleGoogle Scholar
- Guo JW, Zhao TS, Prabhuram J, Wong CW: Preparation and the physical/electrochemical properties of a Pt/C nanocatalyst stabilized by citric acid for polymer electrolyte fuel cells. Electrochim Acta 2005, 50: 1973–1983. 10.1016/j.electacta.2004.09.006View ArticleGoogle Scholar
- Zhang Y, Li G, Wu Y, Luo Y, Zhang L: The formation of mesoporous TiO2spheres via a facile chemical process. J Phys Chem B 2005, 109: 5478–5481. 10.1021/jp0456640View ArticleGoogle Scholar
- Zhu H, Yao K, Zhang H, Yang D: InOOH hollow spheres synthesized by a simple hydrothermal reaction. J Phys Chem B 2005, 109: 20676–20679. 10.1021/jp0511911View ArticleGoogle Scholar
- Liu Y, Zhang X: Effect of calcination temperature on the morphology and electrochemical properties of Co3O4for lithium-ion battery. Electrochim Acta 2009, 54: 4180–4185. 10.1016/j.electacta.2009.02.060View ArticleGoogle Scholar
This article is published under license to BioMed Central Ltd. This is an Open Access article distributed under the terms of the Creative Commons Attribution License (http://creativecommons.org/licenses/by/2.0), which permits unrestricted use, distribution, and reproduction in any medium, provided the original work is properly cited.